Charge density studies in NH~4~[Ti(C~2~O~4~)~2~].2H~2~O crystals at two wavelengths
Sheu, H. S.; Wu, J. C.; Wang, Y.; English, R. B.; Acta Crystallographica Section B 52 (1996) 458–464; doi:10.1107/S0108768195012900

data_2101510
_publ_section_title
;
 Charge density studies in NH~4~[Ti(C~2~O~4~)~2~].2H~2~O crystals at
 two wavelengths
;
_journal_issue                   3
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              458
_journal_page_last               464
_journal_paper_doi               10.1107/S0108768195012900
_journal_volume                  52
_journal_year                    1996
_chemical_formula_moiety         'N1 H4 [Ti (C2 O4 )2 ], 2H2 O'
_chemical_formula_sum            'C4 H8 N O10 Ti'
_chemical_formula_weight         278.1
_space_group_IT_number           181
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P 64 2 (0 0 2)'
_symmetry_space_group_name_H-M   'P 64 2 2'
_atom_type_scat_source           IntTabIV
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            3
_cell_length_a                   8.931(2)
_cell_length_b                   8.931(2)
_cell_length_c                   10.8930(10)
_cell_measurement_reflns_used    24
_cell_measurement_temperature    130
_cell_measurement_theta_max      36
_cell_measurement_theta_min      19
_cell_volume                     752.5(2)
_diffrn_measurement_device       'Nonius CAD4'
_diffrn_measurement_method
;\q/2\q scan width 2(0.70 + 0.35tan\q)\% in 2\q,
speed 2.06 to 8.24\% min^-1^
;
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.032
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_number            20298
_diffrn_reflns_theta_max         60
_diffrn_standards_decay_%        4
_diffrn_standards_interval_time  120
_diffrn_standards_number         3
_exptl_absorpt_coefficient_mu    0.84
_exptl_absorpt_correction_T_max  0.84
_exptl_absorpt_correction_T_min  0.74
_exptl_absorpt_correction_type   'integration from crystal shape'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    1.840
_exptl_crystal_description       'olive shaped'
_exptl_crystal_F_000             423
_exptl_crystal_size_max          0.5
_exptl_crystal_size_mid          0.28
_exptl_crystal_size_min          0.28
_refine_diff_density_max         0.56
_refine_diff_density_min         -0.74
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_obs   2.68
_refine_ls_hydrogen_treatment    'H atoms in calculated positions'
_refine_ls_number_parameters     48
_refine_ls_number_reflns         3170
_refine_ls_R_factor_obs          0.025
_refine_ls_shift/esd_max         0.001
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     'w = 1/[\s^2^(F~o~) + 0.00005F~o~^2^]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_obs         0.024
_reflns_number_observed          3170
_reflns_number_total             3699
_reflns_observed_criterion       I>2\s(I)
_cod_data_source_file            as0695.cif
_cod_data_source_block           as0695b
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'w = 1/[\s^2^(F~o~) +
0.00005F~o~^2^]' was changed to 'calc'. New tag
'_refine_ls_weighting_details' was created. The value of the new tag
was set to 'w = 1/[\s^2^(F~o~) + 0.00005F~o~^2^]'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_original_cell_volume        752.4(2)
_cod_original_formula_sum        'C4 H8 N1 O10 Ti1'
_cod_database_code               2101510